LASER SURFACE PREPARATION OF EPOXY COMPOSITES
FOR SECONDARY BONDING: OPTIMIZATION OF ABLATION
Frank L. Palmieri*, John Hopkins*, Christopher J. Wohl*, Yi Lin, John W. Connell*, Marcus A.
(Tony) Belcher, and Kay Y. Blohowiak
*NASA Langley Research Center, Hampton, VA 2368-2199
National Institute of Aerospace, Hampton, VA 23666 The Boeing Company, Seattle, WA 98124-2207
ABSTRACT Surface preparation has been identified as one of the most critical aspects of attaining predictable
and reliable adhesive bonds. Energetic processes such as laser ablation or plasma treatment are
amenable to automation and are easily monitored and adjusted for controlled surface preparation.
A laser ablation process was developed to accurately remove a targeted depth of resin,
approximately 0.1 to 20 m, from a carbon fiber reinforced epoxy composite surface while
simultaneously changing surface chemistry and creating micro-roughness. This work demonstrates
the application of this process to prepare composite surfaces for bonding without exposing or
damaging fibers on the surface. Composite panels were prepared in an autoclave and had a resin
layer approximately 10 m thick above the fiber reinforcement. These composite panels were laser
surface treated using several conditions, fabricated into bonded panels and hygrothermally aged.
Bond performance of aged, experimental specimens was compared with grit blast surface treated
specimens using a modified double cantilever beam test that enabled accelerated saturation of the
specimen with water. Comparison of bonded specimens will be used to determine how ablation
depth may affect average fracture energies and failure modes.
Aircraft manufacturers rely on adhesive bonding for the assembly of primary structure to improve
performance, reduce costs and meet rigorous safety regulations. Although airframe primary
structures have been assembled with adhesive bonds for over 60 years, bonding technologies
continue to develop rapidly as fiber reinforced plastic (FRP) becomes more prevalent. 1,2 Surface
preparation has been recognized as a critical step to achieving a strong, durable, predictable
adhesive bond. The surface preparation of composites is particularly challenging because of the
broad range of surface conditions that are possible depending on the composite fabrication method
and chemical composition.3 Changes in bond performance can often be attributed to variation in
surface preparation when using manual abrasion.1,4 Also, detecting residual contaminants such as
mold release agents or other materials used during composite fabrication can be challenging.
Energetic techniques such as laser ablation and atmospheric pressure plasma to improve
repeatability and quality of surface preparation are under evaluation by airframe manufacturers.5,6
Preliminary studies by this group and others of laser ablation for surface preparation on both
composites and metals have warranted a more detail understanding of how laser ablation affects
bond performance.7-11 A high fidelity laser ablation process is needed to control the depth of
ablation and avoid exposing or damaging carbon fibers. Composite parts fabricated by various
methods and comprised of dissimilar fiber architectures are likely to have different resin contents
on their surfaces. Thus a thorough understanding of the laser ablation parameters is needed to
account for these differences, in order to sufficiently mature this technology for industrial use. The
depth of penetration into a composite surface during laser ablation is a critical aspect of the surface
preparation and is the subject of this report.
1.1 State-of-the-Art Surface Preparation
For large-scale manufacturing, surface preparation of composites for secondary adhesive bonding
is commonly accomplished by either mechanical abrasion (i.e., sanding, grit blasting) or the
removal of a co-cured fabric known as peel ply.
1.1.1 Mechanical abrasion
Mechanical abrasion techniques such as sanding and grit blasting are labor intensive, difficult to
automate, and are therefore sensitive to operator induced variability. Abrasion processes typically
create debris that must be carefully removed from the faying surface and disposed of before
bonding. When performed correctly, abrasive surface preparation results in strong bonds that have
shown long term stability.12, 13
1.1.2 Peel ply
Peel ply is a layer of fabric that is applied as the final layer in a laminated, composite part before
it is cured. The peel ply layer is removed from the cured composite part to expose a roughened,
clean surface for bonding. Peel plies vary in terms of material composition and application method,
and selection of a peel ply depends heavily on the composite content, molding process, adhesive
type, and planned bonding process. Ideally, peel ply would eliminate the need for mechanical
abrasion, but in some cases abrasion is required after peel ply removal.4, 13
1.2 Laser Surface Preparation
Laser surface preparation is accomplished by ablation, which can be defined as vaporization of
material due to intense laser irradiation. Organic polymer systems generally do not exhibit melting,
re-freezing, and re-deposition processes that may be observed in other materials.6 Ablation has
been used to create high precision surface topography while simultaneously removing surface
contaminants and modifying surface chemistry.6, 8-11 The depth of ablation depends primarily on
the laser fluence and number of passes or pulses directed at a point on the surface.8 The ablation
depth can be controlled by varying the average laser power, which is directly related to the laser
fluence.14 This report investigates the effect of laser power and therefore ablation depth on the
adhesive bond performance of carbon fiber reinforced polymer (CFRP) composites.
1.3 Previously Reported Findings
Previous work from these authors investigated laser ablation to prepare single lap shear specimens
from CFRP substrates. The specimens were subjected to long-term aging at elevated temperature
and humidity before being tested. Although laser power and ablation depth were not variables, it
was found laser power must be monitored to assure repeatable specimen preparation. In this earlier
study, samples prepared using laser ablation showed properties similar to those of control samples
prepared using peel ply.14
1.4 Contents of this Report
The purpose of the current work is to investigate the role of laser power on surface preparation
primarily in terms of ablation depth and subsequent effect on adhesive bond performance after
hygrothermal aging. Modified double cantilever beam specimens were used to enable rapid
saturation of the bondline. Ablation results, contact angle measurements, average fracture energies
(GAVG), and failure mode data are presented.
Composite panels (CFRP, 30.5 cm x 30.5 cm) were prepared from two plies of unidirectional
Torayca P2302-19 prepreg tape (T800H/3900-2 carbon fiber/toughened epoxy resin system) and
cured in an autoclave at 177 C (350 F) and 690 KPa (100 psi). Release from the caul plate was
accomplished using either high temperature polyimide film coated with Zyvax Watershield or by
using Airtech A4000 release film, respectively referred to as Zyvax and fluorinated ethylene
propylene (FEP). Both release methods resulted in a nominally smooth panel surface that released
easily from the mold. Eight-ply panels were fabricated using the same method, but Release Ease
234 TFP (a fluoropolymer-coated cloth from Airtech) was used for mold release, which resulted
in a textured surface. White aluminum oxide grit (180 mesh) was used for grit blasting of control
specimens. Grit blasting was carried out in a non-recycling system with air at 138 kPa (20 psi).
Adhesive used for bonding mechanical test specimens was Hysol EA9696 from Henkel
Corporation with an areal weight of 0.39 kg/m2 (0.08 PSF) on a polyester fiber carrier mat.
2.2 Laser Processing
Laser ablation was performed on a PhotoMachining, Inc. system with a Coherent, Avia,
frequency tripled, Nd:YAG laser (2 W nominal pulsed output at 355 nm). CFRP panels were
ablated with two patterns, according to Table 1, by direct irradiation with a focused beam. The
nominal spot size was 25 m, and the pulse frequency was 80 kHz. Lines, created by a series of
overlapping pulses, were oriented along the fiber direction on each panel such that the ablation
Pattern A was parallel to crack extension during testing. During ablation, the composite part was
held stationary while the laser spot was scanned using a galvanometer. The write speed, 25.4 cm/s
(10 in/s), and pulse frequency, 80 kHz, were held constant for all experiments. The average laser
power was monitored after the final lens element using a thermopile sensor (model 3A-SH) and
Nova II power meter from Ophir Spirocon LLC. The power was tuned to the power levels specified
in Table 1 using a custom beam attenuator from PhotoMachining Inc.
Table 1: Experiment matrix for mechanical test specimen preparation.